Abstract
Natural soft materials harness hierarchy and structures at all scales to build function. Adapting this paradigm to our technological needs, from mechanical, phononic and photonic metamaterials to functional surfaces prompts the development of new fabrication pathways with improved scalability, design flexibility and robustness. Here we show that the inherent periodicity of the Rayleigh–Taylor instability in thin polymeric liquid films can be harnessed to spontaneously fabricate structured materials. The fluidic instability yields pendant drops lattices, which become solid upon curing of the polymer, thereby permanently sculpting the interface of the material. We solve the inverse design problem, taming the instability, so that the structures we form can be tailored, over a range of sizes spanning over two decades. This allinone methodology could potentially be extended down to the scales where continuum mechanics breaks down, while remaining scalable.
Introduction
Capillary effects are ubiquitous in inert and living matter where they dominate the dynamics of fluids at small length scales, in drops, bubbles and thin films^{1}. They are central to various technological applications spanning the fields of chemical engineering, bioengineering, and material science. In their stable limit, capillary effects are routinely used as a method to straighten interfaces, e.g., in the glassfloat process and in coatings on surfaces and fibers^{2,3}, to functionalize surfaces^{4,5}, and to deform or assemble small compliant objects^{6,7,8,9}. Capillary effects also foster the fragmentation of a volume of fluid into a collection of droplets whose radii vary from tenths of nanometers to several millimeters^{10,11,12,13}. These droplets serve as vehicles for biological materials^{14}, for printing polymeric solutions^{15,16}, or are destined to combustion^{17}. However, to this day, interfacial instabilities are rarely seen as a pathway to give spatial order to materials^{13,18,19}. Such structures could find applications in various fields from mechanical, phononic, and photonic metamaterials to functional surfaces^{4,20,21,22}.
Melts and amorphous phases are universally used in manufacturing, given that they can be deformed to take a desired shape, which becomes a tangible object upon solidification. Examples include glass blowing, metal casting, plastic molding, softlithography, and 3D printing^{14,23}. While spatial order arises from applied constraints in these engineered structures, patterns in nature often capitalize on the inherent periodicity and robustness of instabilities^{24}.
Here, we show that the Rayleigh–Taylor instability in thin polymer films can be harnessed at the materials level to spontaneously shape solid structures. Specifically, thin liquid elastomeric coatings are destabilized to generate dropshaped smooth structures with tailored geometrical properties, which are predicted by the theoretical framework we introduce. As the elastomer cures, these fluidmediated structures yield an elastic material. We show that the robustness of the instability across length scales, and material properties are instrumental in making this passive methodology a scalable fabrication pathway.
Results
Tailoring the Rayleigh–Taylor instability
Figure 1a outlines our approach: a liquid elastomeric polymer (polydimetylsiloxane PDMS Sylgard 184, Dow Corning) is coated on the outside of a cylinder with radius R. The substrate is then rotated at speed Ω, either in a lathe or in a centrifuge depending on the targeted acceleration a = RΩ^{2} (see Methods). We observe the destabilization of the interface of the film into a lattice of drops. As the polymer cures, the array of liquid drops solidifies, thereby permanently sculpting this initially fluid system (Fig. 1b). The resulting structure can be used as a network, or the drops may be peeled off from the substrate and used individually (Fig. 1c), making of this method an inherently scalable fabrication pathway.
The Rayleigh–Taylor instability (RTI) in thin liquid films describes the destabilization of a fluid interface under the action of surface tension, viscous stresses and an acceleration field, usually gravity^{25,26}. The drops shown in Fig. 1b, which serve as a reference case, originate from the linearly most unstable mode of the RTI in a thin film subject to the destabilizing action of gravity. The wavelength of the pattern is \(\lambda _{\mathrm{M}} = 2\pi \sqrt 2 \ell _{\mathrm{c}}\), where \(\ell _{\mathrm{c}}\) is the capillary length^{25}. This characteristic length is obtained by balancing gravity and capillary effects so that \(\ell _{\mathrm{c}} = \sqrt {\gamma /\rho g}\), where γ is the surface tension of the liquid, ρ its density and g is the acceleration of gravity (viscous effects only enter in setting the time scale of the instability). While gravity yields centrimetric droplets (\(\ell _{\mathrm{c}} = 1.45\) mm for PDMS so that \(\lambda _{\mathrm{M}} \simeq 13\,{\mathrm{mm}}\)), smaller scales can be reached with the larger acceleration fields we generate via centrifugation. Typical results are shown in Fig. 1d and e, corresponding to accelerations RΩ^{2} = 10.2g and a = 1421g, respectively. In our experiments, we define the location of a drop by the coordinate of its apex. We then use this data to generate a Voronoi diagram with partitions of mean area \({\cal S}\) (inset of Fig. 1f). We define the wavelength of the lattice as \(\lambda = 4/3^{1/4}\sqrt {\cal S}\). The prefactor corresponds to an ideal regular hexagonal lattice for which \({\cal S} = \sqrt {3/4} \lambda ^2\). In Fig. 1f, we show that our experiments collapse on a curve defined by:
where R is the radius of rotation and Ω the rotation speed. Equation 1 matches the classical expression of the most unstable mode of the RTI when substituting a = RΩ^{2} for g, thereby showing that the physics of the instability is unchanged over five decades of accelerations. We find that an acceleration ranging between g and 3 × 10^{4}g yields drops with wavelength ranging from 10 mm to 50 μm, showing the robustness of the instability across length scales (see Fig. 1g–i). For accelerations larger than 10^{3}g (triangles in Fig. 1f), we worked with silicon wafers, which were flat, so that the centrifugal forces is not uniform across the sample. This effect leads to a competition between droplets and rivulets^{27}.
With the above results in hand, it is thus possible to program the instability to obtain a drop lattice with wavelength ranging over three decades, simply by modulating the magnitude of the acceleration field. The drops are remarkably similar across lengthscales as evident from Fig. 1j, where our montage is realized by rescaling each drop by \(\ell = \sqrt {\gamma /\rho R\Omega ^2}\), the generalized capillary length. We anticipate that larger accelerations will produce a similar trend until other effects such as surface roughness or intermolecular forces become appreciable. We now focus on the case where a = g, and investigate thin polymeric films coated on the underside of horizontal substrates.
From instability to order
We examine the regularity of the lattice that emerges spontaneously from the RTI. As the lattice cures, we are able to investigate its geometric properties with ease. In Fig. 2a, we show photographs of the caustics obtained when illuminating the translucent samples with a point source. The starlike shapes in Fig. 2a show the position of the apex of each drop, while the white segments evidence a network of flat valleys in the films separating neighboring droplets^{28}. We construct the Voronoi tessellation using the drops positions, which we show in Fig. 2b. We find that the Voronoi cell boundaries coincide with the film valleys. Each drop may be seen as an isolated system, which has drained the volume initially occupying its tile. There is a majority of hexagons (blue) as well as some pentagons (green) and some heptagons (red). The lattice is thus irregular, albeit composed of tiles of approximatively the same size. Irregularities are inherent to the instability that starts from the edge of the film^{25,26} and progressively invades the sample, accumulating defects, and geometrical frustrations.
To bypass this effect and improve the monodispersity of the drops, we carefully design a layout of surface defects on the substrate. Cylindrical holes (diameter 2 mm, depth 1.6 mm), regularly spaced, are etched on the substrate (Fig. 2c, d). They are used as seed perturbations to trigger the instability simultaneously across the sample. In Fig. 2c and d, we show the results obtained with a square and a hexagonal seed layout with wavelength λ = λ_{M}. The drops are not centered on the defects, but instead are located as far as possible from them, i.e., on the vertices of the dual graph of the seeds pattern. As evident from Fig. 2c and d, we are able to organize the lattice of droplets and tailor the geometry of the unit cell.
The topography of the resulting droplets pattern was digitized using a 3D laser scanner (NextEngine). Data are reported in Fig. 2e and f and colorcoded such that drops apex appear in red and valleys in blue. The small cylindrical cavities evident in Fig. 2c and d mark the location of the seeds. The initial film flowed away from the seeds in a direction parallel to the sample^{25} to feed off the neighboring drops. In the classical RTI (no seeds, uniform initial coating), the growth rate of drops in a square pattern is lower than that of a hexagonal arrangement—such that square lattices are usually not observed unless forced^{25}. The forcing achieved through the seeds that have been laid out in a square lattice, appears to be sufficient to promote this pattern. Note that in both the square and the hexagonal cases, we observe that the regularity of the lattice comes along with a degree of uniformity of the drops amplitude. We now aim to elucidate the underlying mechanisms that set the amplitude and the shape of these drops.
Inverse design
In Fig. 3a, we report the final amplitude of drops for substrates coated with the same initial film thickness (h_{0} = 270 μm), while the work time τ_{w} at which the substrates are inverted is varied. The work time τ_{w} denotes the time interval between the preparation of the polymer, i.e., when curing begins, and the time at which the sample is inverted, i.e., when the gravity induced flow begins. The amplitude of the drops is averaged on 75 drops across each sample. For small values of τ_{w} (here τ_{w} < 2000 s), the final drop amplitude is independent of τ_{w}. However, for larger values of τ_{w} smaller drops are obtained. We now turn to rationalize this dependance.
In our problem, the final state of the film is the result of the competition between two time scales. First, the RTI initially grows exponentially with characteristic time τ_{i} = 12τ_{v}, where \(\tau _{\mathrm{v}} = \mu \ell _{\mathrm{c}}^4/(\sigma h_{\mathrm{0}}^3)\) is the time scale of drainage in the thin film surrounding the drops^{28}. Note that this time scale strongly depends on h_{0}, such that small differences in h_{0} yield large differences in τ_{i}. Second, the elastomer undergoes crosslinking and cures with characteristic time τ_{c}^{29}. We aim to work with physical parameters such that \(\tau _{\mathrm{c}} \gg \tau _{\mathrm{i}}\). To illustrate this time scale separation, we superimpose in Fig. 3b the dynamics of the drop growth, measuring the transmittance of the PDMS coating colored with a black dye, and the time evolution of the polymer viscosity, for a constant shear rate \(\dot \gamma = 0.1\,{\mathrm{s}}^{  1}\). We find that the predicted time scale τ_{i} (black line in Fig. 3b) captures the exponential growth of the instability in our experiments, which saturates in a time (700 s) significantly smaller than curing time (3500 s). Saturation is imparted by the increasing difficulty to drain fluid from the flat regions inbetween the drops (as their thickness decreases). By choosing the initial thickness of the coating, we manage to operate in a regime where the time scales of the problem are separated: first the drops form and then the curing of the polymer solidifies the drops.
At large times, \(t \gg \tau _{\mathrm{i}}\), and before curing \(t \ll \tau _{\mathrm{c}}\) the system consists of a series of drops surrounded by thin depleted films^{28}. Asymptotic analysis of the equations governing this creeping flow reveals that perturbations to the drops shape relax much faster than the intervening region between drops can drain^{28}. As a result, the drops are in nearequilibrium and their shape may be derived with a quasistatic approach matched asymptotically to a surrounding much thinner film. The geometry of the drops is characterized by θ(s) as defined in inset of Fig. 4a, such that the tangent to the interface is r′(s) = (cos(θ(s)), sin(θ(s))), where a prime denotes a differentiation with respect to the arclength s. Given the symmetry of the problem, we search for constantpressure solutions of
obtained by balancing gravity and surface tension effects. Integration of this equation subject to the adequate set of boundary conditions (x(0) = 0 and θ(0) = 0) is performed using a shooting algorithm leveraging on the symmetry of the problem so that the tangent to the drop is horizontal when crossing the x − axis (at the appex). Results obtained via this method are shown in Fig. 4a. The family of solutions are colorcoded such that solutions of lesser amplitude (and volume) are marked in blue and solutions of larger amplitudes are indicated in red. All solutions are recast in Fig. 4b as a function of their dimensionless amplitude \(A/\ell _{\mathrm{c}}\) and the dimensionless coating thickness \(h_{\mathrm{0}}/\ell _{\mathrm{c}}\) required to form them (assuming a hexagonal arrangement of the drops to evaluate their volume, and neglecting the volume of fluid in the connecting films). The solution branch in Fig. 4b is multivalued and presents a fold separating stable solutions (small values of A) and unstable ones (large values of A, thus never observed in experiments) from regions where no static solutions exist (large values of h_{0}). The foldpoint in the curve corresponds to the drop presented as a dashed line in Fig. 4a, such that only the shapes below this curve are expected to be found in our experiments as we show next.
The amplitudes of the droplets obtained in our experiments for different initial coating thickness h_{0} are averaged across the sample and plotted in Fig. 4b as red triangles. To estimate the volume of PDMS trapped in the seed, we weigh the drops after peeling from the sample and recast their volume in terms of h_{0} using a hexagonal lattice. In Fig. 4c–h, we present photographs of crosssectional cuts of the solidified elastic drops along with the axisymmetric solutions of the drop shapes that best fit them. We find a favorable agreement between theory and experiments. Figure 4h is the largest drop that can be obtained experimentally. Increasing the thickness of the initial film coating further leads to dripping, as no equilibrium solution exists (foldpoint). The shape of the elastic interface is thus rationalized using arguments and an equation that belongs to the realm of fluid mechanics. Such a predictive model allows us to quantitatively solve the inverse problem: the targeted shape dictates the initial conditions, chosen using the explicit relation plotted in Fig. 4b. Similar arguments apply in the context of our centrifuged experiments. The targeted scale, λ, sets the acceleration and radius obtained reversing Eq. 1. Drop shapes are then obtained substituting the generalized capillary length \(\ell = \sqrt {\gamma /\rho R\Omega ^2}\) for \(\ell _{\mathrm{c}}\) in Fig. 4b. Drops with identical dimensionless volume indeed collapse on the predicted shape as shown in Fig. 1j.
Complex elastic surfaces
At smaller scale, precisely controlling the surface defect on the substrate and the initial thickness is more challenging. We propose an alternative approach. We start with a smooth substrate, which we coat and rotate to generate an imperfect drop lattice. We then use this lattice as a substrate, which is coated and rotated again at the same speed. Each time, the previously obtained lattice serves to force the instability. After a few generations, we find that the shapes that we obtain converge towards the same aspect ratio. In Fig. 5a, we show the hairy elastic structures obtained after 16 generations of coating at an acceleration RΩ^{2}/g = 404.
We then take advantage of the elastic properties of our materials and show that those structures can be dynamically actuated into a variety of convex and concave shapes. Under pressure loading, a hexagonal array of droplets with regular amplitude bulges to form a dimpled sphere (Fig. 5b and Supplementary Movie 1). This deformation is reversible owing to the constitutive properties of the elastomer. Similar deformations are obtained for hairy surfaces (Fig. 5c and Supplementary Movie 2) at an intermediate scale. At microscopic scale, twotier controlled structures are demonstrated on surfaces permanently deformed with positive and negative Gaussian curvature and imaged with SEM (Fig. 5d, e). An additional wrinkle morphology at the surface of the structure is observed for larger values of the acceleration (RΩ^{2}/g = 1.2 × 10^{4}) with the multiple coating approach (Fig. 5f). The last layer cures on a substrate which is elastically deformed due to the acceleration field. When the centrifugation is stopped after curing, the substrate relaxes so that the last layer is under compression and the thin film wrinkles^{30}.
Discussion
We have proposed and characterized a passive methodology that freezes an instability at a stage between a compact macroscopic liquid volume and its subsequent dispersion into drops, so as to harness the resulting structure. We have shown that the RTI in polymer films can be rationalized and tamed to tailor the resulting structures. The final structure is elastic, albeit its morphology is underpinned by a combination of fluidic processes: first an instability and then a quasistatic equilibrium. Timing and initial conditions allowed us to control the drop amplitudes, and seeds fostered uniform lattices. While centimeter drops are the norm, we have demonstrated that much smaller scales are attainable, so that this method could be used in the microfabrication of soft materials with applications to optics or acoustics, or to control surface properties such as adhesion and wetting. Our method furthers our capacities in fastprototyping complementing additive manufacturing and other conventional molding techniques. We expect that our approach can be extended to other liquids, which react or undergo a phase transition (other polymers, inks, wax, molten glass, and metals) and other instabilities, therefore opening the way to fabricate a broader repertoire of shapes.
Methods
Experimental procedure
Vinylpolysiloxane (VPS) or polydimetylsiloxane (PDMS) were used for the layer fabrication and, for both cases, curing was performed at room temperature (20 °C). For PDMS (Sylgard 184, Dow Corning), the base and curing agent were mixed in a weight ratio of 10:1 using a centrifugal mixer (ARE310, Thinky) for 30 s at 2000 rpm (clockwise), and then for 30 s at 2200 rpm (counterclockwise). The curing process was sped up by adding an accelerator (36559, Dow Corning) to the PDMS, with a weight ratio of 5:1 (PDMSbase to cureaccelerator). VPS (Elite Double 32, Zhermack) was mixed with a weight ratio of 1:1 (base to curing agent) using a centrifugal mixer for 10 s at 2000 rpm (clockwise), and then 10 s at 2200 rpm (counterclockwise). A larger gravity field was emulated either in a lathe (radii of gyration R = [57,83.8] mm, rotation speeds Ω = [16.5, 21.9, 34.6,68.9, 102.7] rad s^{−1}), in a centrifuge (Sorvall RT6000d, R = 110 mm, Ω = [104.7, 157.1, 261.8, 314.2, 356.0] rad s^{−1}), in a spincoater (Laurell WS650 R = 63.5 mm, rotation speeds Ω = 80–1200 rad s^{−1}) or in a superspeed centrifuge (Sorvall Lynx4000, R = 65 mm, rotation speeds Ω = [523.6, 733.0, 1256, 1571, 1885, 2094] rad s^{−1}). To trigger the instability, an array of square or hexagonal holes (diameter 2 mm, length scale λ) was lasercut in an acrylic plate (thickness 1.6 mm) glued on the substrate. The VPS and PDMS solutions were then spincoated (Laurell WS650) on the acrylic plate to produce uniform layers of initial thickness in the range 150 ≤ h[μm] ≤ 590. The topography of the resulting droplets patterns was digitized using a 3D laser scanner (NextEngine) and the data were postprocessed using an inhouse Matlab code to quantify the lattice order, length scale, and amplitude of the droplets in the lattice. The microscopic droplets were imaged with a Scanning Electron Microscope Philips XL 30 SEMFEG. The dynamics of the drop growth was measured by mixing a black dye (SilcPig, Smoothon with a dye concentration of 0.1% in mass) in the PDMS suspension prior to curing using the BeerLambert law that relates the transmittance to the thickness and dye concentration^{31}. The viscosity of the PDMS polymer solution was characterized with a rheometer (ARG2, TA Instruments) as a function of time and at a constant temperature (20 °C). The shear rate was fixed at \(\dot \gamma \sim u/h\sim 0.1\) s^{−1}, consistent with the characteristic drainage velocity and film thickness.
Data availability
The authors declare that the data supporting the findings of this study are available within the paper and its Supplementary Information Files.
References
De Gennes, P.G., BrochardWyart, F. & Quéré, D. Capillarity and Wetting Phenomena: Drops, Bubbles, Pearls, Waves (Springer, New York, NY, 2013).
Pilkington, L. A. B. Review lecture. the float glass process. Proc. R. Soc. A 314, 1–25 (1969).
Kistler, S. F. & Schweizer, P. M. Liquid Film Coating (Chapman Hall, London, 1997).
Lafuma, A. & Quéré, D. Superhydrophobic states. Nat. Mater. 2, 457 (2003).
Tuteja, A. et al. Designing superoleophobic surfaces. Science 318, 1618–1622 (2007).
Huang, J. et al. Capillary wrinkling of floating thin polymer films. Science 317, 650–653 (2007).
Jerison, E. R., Xu, Y., Wilen, L. A. & Dufresne, E. R. Deformation of an elastic substrate by a threephase contact line. Phys. Rev. Lett. 106, 186103 (2011).
Whitesides, G. M. & Grzybowski, B. Selfassembly at all scales. Science 295, 2418–2421 (2002).
Pokroy, B., Kang, S. H., Mahadevan, L. & Aizenberg, J. Selforganization of a mesoscale bristle into ordered, hierarchical helical assemblies. Science 323, 237–240 (2009).
Villermaux, E. Fragmentation. Annu. Rev. Fluid. Mech. 39, 419–446 (2007).
Squires, T. M. & Quake, S. R. Microfluidics: fluid physics at the nanoliter scale. Rev. Mod. Phys. 77, 977 (2005).
Baroud, C. N., Gallaire, F. & Dangla, R. Dynamics of microfluidic droplets. Lab. Chip. 10, 2032–2045 (2010).
Kaufman, J. J. et al. Structured spheres generated by an infibre fluid instability. Nature 487, 463–467 (2012).
Whitesides, G. M. The origins and the future of microfluidics. Nature 442, 368 (2006).
de Gans, B.J., Duineveld, P. C. & Schubert, U. S. Inkjet printing of polymers: state of the art and future developments. Adv. Mater. 16, 203–213 (2004).
McKinley, G. H. Viscoelastocapillary thinning and breakup of complex fluids. Rheol. Rev. 3, 1–48 (2005).
Bayvel, L. & Orzechowski, Z. Liquid Atomization. (Taylor & Francis, Washington, DC, 1993).
Srinivasarao, M., Collings, D., Philips, A. & Patel, S. Threedimensionally ordered array of air bubbles in a polymer film. Science 292, 79–83 (2001).
Islam, Tu & Gandhi, P. S. Fabrication of multscale fractallike structures by controlling fluid interface instability. Sci. Rep. 6, 37187 (2016).
Kolle, M. et al. Mimicking the colourful wing scale structure of the papilio blumei butterfly. Nat. Nanotechnol. 5, 511–515 (2010).
Wang, P., Casadei, F., Shan, S., Weaver, J. C. & Bertoldi, K. Harnessing buckling to design tunable locally resonant acoustic metamaterials. Phys. Rev. Lett. 113, 014301 (2014).
Coulais, C., Teomy, E., de Reus, K., Shokef, Y. & van Hecke, M. Combinatorial design of textured mechanical metamaterials. Nature 535, 529–532 (2016).
Truby, R. L. & Lewis, J. A. Printing soft matter in three dimensions. Nature 540, 371–378 (2016).
Gallaire, F. & Brun, P.T. Fluid dynamic instabilities: theory and application to pattern forming in complex media. Philos. Trans. R. Soc. A 375, 20160155 (2017).
Fermigier, M., Limat, L., Wesfreid, J., Boudinet, P. & Quilliet, C. Twodimensional patterns in Rayleigh–Taylor instability of a thin layer. J. Fluid. Mech. 236, 349–383 (1992).
Limat, L. et al. Gravitational instabilities of thin liquid layers: dynamics of pattern selection. Phys. D. 61, 166–182 (1992).
Balestra, G., Kofman, N., Brun, P.T., Scheid, B. & Gallaire, F. Threedimensional Rayleigh–Taylor instability under a unidirectional curved substrate. J. Fluid. Mech. 837, 19–47 (2018).
Lister, J. R., Rallison, J. M. & Rees, S. J. The nonlinear dynamics of pendent drops on a thin film coating the underside of a ceiling. J. Fluid. Mech. 647, 239–264 (2010).
Lee, A. et al. Fabrication of slender elastic shells by the coating of curved surfaces. Nat. Commun. 7, 11155 (2016).
Bowden, N., Brittain, S., Evans, A. G., Hutchinson, J. W. & Whitesides, G. M. Spontaneous formation of ordered structures in thin films of metals supported on an elastomeric polymer. Nature 393, 146 (1998).
López Jiménez, F., Kumar, S. & Reis, P. M. Soft color composites with tunable optical transmittance. Adv. Opt. Mater. 4, 620–626 (2016).
Acknowledgments
We thank José L. Avalos for experimental support.
Author information
Authors and Affiliations
Contributions
P.T.B., P.M.R., and J.M. designed the research. P.T.B. supervised the project. J.M., E.F.S., and P.T.B. performed experiments and analyzed data. All authors contributed to interpret experimental observations. P.T.B., J.M., and P.M.R. wrote paper.
Corresponding author
Ethics declarations
Competing interests
The authors declare no competing interests.
Additional information
Publisher’s note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Electronic supplementary material
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Marthelot, J., Strong, E.F., Reis, P.M. et al. Designing soft materials with interfacial instabilities in liquid films. Nat Commun 9, 4477 (2018). https://doi.org/10.1038/s41467018069847
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/s41467018069847
This article is cited by

Capillary forces generated by biomolecular condensates
Nature (2022)

Stability Analysis of Miscible Viscous Fingering in Bingham and Carreau Fluids
Transport in Porous Media (2022)

Aqueous TwoPhase Interfacial Assembly of COF Membranes for Water Desalination
NanoMicro Letters (2022)

Stabilization of liquid instabilities with ionized gas jets
Nature (2021)

Bubble casting soft robotics
Nature (2021)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.